Presentation on theme: "Chapter 15 - 1 Chapter 15: Characteristics, Applications & Processing of Polymers ISSUES TO ADDRESS... What are the tensile properties of polymers and."— Presentation transcript:
Chapter Chapter 15: Characteristics, Applications & Processing of Polymers ISSUES TO ADDRESS... What are the tensile properties of polymers and how are they affected by basic microstructural features ? Hardening, anisotropy, and annealing in polymers. How does the elevated temperature mechanical response of polymers compare to ceramics and metals? What are the primary polymer processing methods?
Chapter Mechanical Properties of Polymers – Stress-Strain Behavior Fracture strengths of polymers ~ 10% of those for metals Deformation strains for polymers > 1000% – for most metals, deformation strains < 10% brittle polymer plastic elastomer elastic moduli – less than for metals Adapted from Fig. 15.1, Callister & Rethwisch 8e.
Chapter Mechanisms of Deformation—Brittle Crosslinked and Network Polymers brittle failure plastic failure (MPa) x x aligned, crosslinked polymer Stress-strain curves adapted from Fig. 15.1, Callister & Rethwisch 8e. Initial Near Failure Initial network polymer Near Failure
Chapter Mechanisms of Deformation — Semicrystalline (Plastic) Polymers brittle failure plastic failure (MPa) x x crystalline block segments separate fibrillar structure near failure crystalline regions align onset of necking undeformed structure amorphous regions elongate unload/reload Stress-strain curves adapted from Fig. 15.1, Callister & Rethwisch 8e. Inset figures along plastic response curve adapted from Figs & 15.13, Callister & Rethwisch 8e. (15.12 & are from J.M. Schultz, Polymer Materials Science, Prentice- Hall, Inc., 1974, pp )
Chapter Predeformation by Drawing Drawing…(ex: monofilament fishline) -- stretches the polymer prior to use -- aligns chains in the stretching direction Results of drawing: -- increases the elastic modulus (E) in the stretching direction -- increases the tensile strength (TS) in the stretching direction -- decreases ductility (%EL) Annealing after drawing decreases chain alignment -- reverses effects of drawing (reduces E and TS, enhances %EL) Contrast to effects of cold working in metals! Adapted from Fig , Callister & Rethwisch 8e. (Fig is from J.M. Schultz, Polymer Materials Science, Prentice-Hall, Inc., 1974, pp )
Chapter Compare elastic behavior of elastomers with the: -- brittle behavior (of aligned, crosslinked & network polymers), and -- plastic behavior (of semicrystalline polymers) (as shown on previous slides) Stress-strain curves adapted from Fig. 15.1, Callister & Rethwisch 8e. Inset figures along elastomer curve (green) adapted from Fig , Callister & Rethwisch 8e. (Fig is from Z.D. Jastrzebski, The Nature and Properties of Engineering Materials, 3rd ed., John Wiley and Sons, 1987.) Mechanisms of Deformation— Elastomers (MPa) initial: amorphous chains are kinked, cross-linked. x final: chains are straighter, still cross-linked elastomer deformation is reversible (elastic)! brittle failure plastic failure x x
Chapter Thermoplastics: -- little crosslinking -- ductile -- soften w/heating -- polyethylene polypropylene polycarbonate polystyrene Thermosets: -- significant crosslinking (10 to 50% of repeat units) -- hard and brittle -- do NOT soften w/heating -- vulcanized rubber, epoxies, polyester resin, phenolic resin Adapted from Fig , Callister & Rethwisch 8e. (Fig is from F.W. Billmeyer, Jr., Textbook of Polymer Science, 3rd ed., John Wiley and Sons, Inc., 1984.) Thermoplastics vs. Thermosets Callister, Fig T Molecular weight TgTg TmTm mobile liquid viscous liquid rubber tough plastic partially crystalline solid crystalline solid
Chapter Decreasing T increases E -- increases TS -- decreases %EL Increasing strain rate same effects as decreasing T. Adapted from Fig. 15.3, Callister & Rethwisch 8e. (Fig is from T.S. Carswell and J.K. Nason, 'Effect of Environmental Conditions on the Mechanical Properties of Organic Plastics", Symposium on Plastics, American Society for Testing and Materials, Philadelphia, PA, 1944.) Influence of T and Strain Rate on Thermoplastics ºC 20ºC 40ºC 60ºC to 1.3 (MPa) Plots for semicrystalline PMMA (Plexiglas)
Chapter Melting & Glass Transition Temps. What factors affect T m and T g ? Both T m and T g increase with increasing chain stiffness Chain stiffness increased by presence of 1.Bulky sidegroups 2.Polar groups or sidegroups 3.Chain double bonds and aromatic chain groups Regularity of repeat unit arrangements – affects T m only Adapted from Fig , Callister & Rethwisch 8e.
Chapter 15 - Representative T g values ( C): PE (low density) PE (high density) PVC PS PC Selected values from Table 15.2, Callister & Rethwisch 8e. 10 Stress relaxation test: -- strain in tension to o and hold. -- observe decrease in stress with time. Relaxation modulus: Time-Dependent Deformation time strain tensile test oo s(t) There is a l arge decrease in E r for T > T g. (amorphous polystyrene) Adapted from Fig. 15.7, Callister & Rethwisch 8e. (Fig is from A.V. Tobolsky, Properties and Structures of Polymers, John Wiley and Sons, Inc., 1960.) rigid solid (small relax) transition region T(ºC) TgTg E r (10 s) in MPa viscous liquid (large relax)
Chapter Crazing During Fracture of Thermoplastic Polymers fibrillar bridges microvoids crack aligned chains Adapted from Fig. 15.9, Callister & Rethwisch 8e. Craze formation prior to cracking – during crazing, plastic deformation of spherulites – and formation of microvoids and fibrillar bridges
Chapter Polymer Formation There are two types of polymerization –Addition (or chain) polymerization –Condensation (step) polymerization
Chapter Polymer Additives Improve mechanical properties, processability, durability, etc. Fillers –Added to improve tensile strength & abrasion resistance, toughness & decrease cost –ex: carbon black, silica gel, wood flour, glass, limestone, talc, etc. Plasticizers – Added to reduce the glass transition temperature T g below room temperature – Presence of plasticizer transforms brittle polymer to a ductile one – Commonly added to PVC - otherwise it is brittle
Chapter Polymer Additives (cont.) Stabilizers –Antioxidants –UV protectants Lubricants – Added to allow easier processing – polymer “slides” through dies easier – ex: sodium stearate Colorants – Dyes and pigments Flame Retardants – Substances containing chlorine, fluorine, and boron
Chapter Processing of Plastics Thermoplastic –can be reversibly cooled & reheated, i.e. recycled –heat until soft, shape as desired, then cool –ex: polyethylene, polypropylene, polystyrene. Thermoset – when heated forms a molecular network (chemical reaction) – degrades (doesn’t melt) when heated – a prepolymer molded into desired shape, then chemical reaction occurs – ex: urethane, epoxy
Chapter Processing Plastics – Compression Molding Thermoplastics and thermosets polymer and additives placed in mold cavity mold heated and pressure applied fluid polymer assumes shape of mold Fig , Callister & Rethwisch 8e. (Fig is from F.W. Billmeyer, Jr., Textbook of Polymer Science, 3rd ed., John Wiley & Sons, 1984.)
Chapter Processing Plastics – Injection Molding Fig , Callister & Rethwisch 8e. (Fig is from F.W. Billmeyer, Jr., Textbook of Polymer Science, 2nd edition, John Wiley & Sons, 1971.) Thermoplastics and some thermosets when ram retracts, plastic pellets drop from hopper into barrel ram forces plastic into the heating chamber (around the spreader) where the plastic melts as it moves forward molten plastic is forced under pressure (injected) into the mold cavity where it assumes the shape of the mold Barrel
Chapter Processing Plastics – Extrusion Fig , Callister & Rethwisch 8e. (Fig is from Encyclopædia Britannica, 1997.) thermoplastics plastic pellets drop from hopper onto the turning screw plastic pellets melt as the turning screw pushes them forward by the heaters molten polymer is forced under pressure through the shaping die to form the final product (extrudate)
Chapter Processing Plastics – Blown-Film Extrusion Fig , Callister & Rethwisch 8e. (Fig is from Encyclopædia Britannica, 1997.)
Chapter Polymer Types – Fibers Fibers - length/diameter >100 Primary use is in textiles. Fiber characteristics: –high tensile strengths –high degrees of crystallinity –structures containing polar groups Formed by spinning – extrude polymer through a spinneret (a die containing many small orifices) – the spun fibers are drawn under tension – leads to highly aligned chains - fibrillar structure
Chapter Polymer Types – Miscellaneous Coatings – thin polymer films applied to surfaces – i.e., paints, varnishes –protects from corrosion/degradation –decorative – improves appearance –can provide electrical insulation Adhesives – bonds two solid materials (adherands) – bonding types: 1. Secondary – van der Waals forces 2. Mechanical – penetration into pores/crevices Films – produced by blown film extrusion Foams – gas bubbles incorporated into plastic
Chapter Advanced Polymers Molecular weight ca. 4 x 10 6 g/mol Outstanding properties –high impact strength –resistance to wear/abrasion –low coefficient of friction –self-lubricating surface Important applications –bullet-proof vests –golf ball covers –hip implants (acetabular cup) UHMWPE Adapted from chapter- opening photograph, Chapter 22, Callister 7e. Ultrahigh Molecular Weight Polyethylene (UHMWPE)
Chapter Advanced Polymers styrene butadiene Thermoplastic Elastomers Styrene-butadiene block copolymer hard component domain soft component domain Fig , Callister & Rethwisch 8e. (Fig adapted from the Science and Engineering of Materials, 5th Ed., D.R. Askeland and P.P. Phule, Thomson Learning, 2006.) Fig (a), Callister & Rethwisch 8e.
Chapter Limitations of polymers: -- E, y, K c, T application are generally small. -- Deformation is often time and temperature dependent. Thermoplastics (PE, PS, PP, PC): -- Smaller E, y, T application -- Larger K c -- Easier to form and recycle Elastomers (rubber): -- Large reversible strains! Thermosets (epoxies, polyesters): -- Larger E, y, T application -- Smaller K c Table 15.3 Callister & Rethwisch 8e: Good overview of applications and trade names of polymers. Summary